Home > Documents > Mechanical Properties of Materials.pdf

# Mechanical Properties of Materials.pdf

Date post: 02-Jun-2018
Category:
View: 233 times

of 17

Transcript
• 8/10/2019 Mechanical Properties of Materials.pdf

1/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-1

Mechanical Properties of Materials

Material Model

StressesStrains

Learning objectives

Understand the qualitative and quantitative description of mechanical

properties of materials.

Learn the logic of relating deformation to external forces.

• 8/10/2019 Mechanical Properties of Materials.pdf

2/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-2

Tension Test

doLo+

P

P

Tension Test MachineTension-testSpecimens

Lo

L

o

------= PA

o

------ P

do2

4----------------= =

Ultimate Stressu

Rupturef Fracture Stress

p

g

ng

Plastic StrainNormal Strain

NormalStress

AB

C

D

E

FO

Proportional Limit

G

Offset strain

H

I

Elastic Strain

Total Strain

y Offset Yield StressLo

• 8/10/2019 Mechanical Properties of Materials.pdf

3/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-3

Definitions

The point up to which the stress and strain are linearly related is called

the proportional limit.

The largest stress in the stress strain curve is called the ultimate stress. The stress at the point of rupture is called the fracture or rupturestress.

The region of the stress-strain curve in which the material returns to

the undeformed state when applied forces are removed is called the

elastic region.

The region in which the material deforms permanently is called the

plastic region.

The point demarcating the elastic from the plastic region is called the

yield point. The stress at yield point is called the yield stress. The permanent strain when stresses are zero is called the plastic strain.

The off-set yieldstress is a stress that would produce a plastic strain

corresponding to the specified off-set strain.

A material that can undergo large plastic deformation before fracture

is called a ductile material.

A material that exhibits little or no plastic deformation at failure is

called a brittle material.

Hardnessis the resistance to indentation. The raising of the yield point with increasing strain is called strain

hardening.

The sudden decrease in the area of cross-section after ultimate stress is

called necking.

• 8/10/2019 Mechanical Properties of Materials.pdf

4/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-4

Material Constants

Normal Strain

NormalStress

O

Slop

e=Es

Slope=

Et

A

E = Modulus of Elasticity

Es = Secant Modulus at B

Et= Tangent Modulus at B

Slo

pe=

E

B

E= -----------------Hookes Law E Youngs Modulusor Modulus of Elasticity

Poissons ratio: lateral

longitudnal

------------------------------

=

G=G is called the Shear Modulus of Elasticityor the

Modulus of Rigidity

• 8/10/2019 Mechanical Properties of Materials.pdf

5/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-5

3.23 A circular bar of length 6 inch and diameter of 1 inch is made

from a material with a Modulus of Elasticity of E=30,000 ksi and a Pois-

sons ratio of=1/3. Determine the change in length and diameter of thebar when a force of 20 kips is applied to the bar.

• 8/10/2019 Mechanical Properties of Materials.pdf

6/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-6

3.27 An aluminum rectangular bar has a cross-section of

25 mm x 50 mm and a length of 500 mm. The Modulus of Elasticity of

E = 70 GPa and a Poissons ratio of= 0.25. Determine the percentagechange in the volume of the bar when an axial force of 300 kN is applied

to the bar.

• 8/10/2019 Mechanical Properties of Materials.pdf

7/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-7

Logic in structural analysis

Eq

uilibriu

m

Material

Mod

els

Static Equivalency

2

1

3

4

Kinematics

StressesInternal Forcesand Moments

External Forcesand Moments

Strains

Displacements

• 8/10/2019 Mechanical Properties of Materials.pdf

8/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-8

3.43 A roller slides in a slot by the amount P= 0.25 mm in thedirection of the force F. Both bars have an area of cross-section of

A = 100 mm2and a Modulus of Elasticity E = 200 GPa. Bar AP and BP

have lengths of LAP

= 200 mm and LBP

= 250 mm respectively. Determine

the applied force F.

P

F

75o30o

A

B

Fig. P3.43

• 8/10/2019 Mechanical Properties of Materials.pdf

9/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-9

3.46 A gap of 0.004 inch exists between the rigid bar and bar A

before the force F is applied as shown in Figure 3.46. The rigid bar is

hinged at point C. Due to force F the strain in bar A was found to be

- 500 in/in. The lengths of bar A and B are 30 and 50 inches respec-

tively. Both bars have an area of cross-section A= 1 in2and Modulus ofElasticity E = 30,000 ksi. Determine the applied force F.

B

A24 in 36 in

75o

F60 in

C

Fig. P3.46

• 8/10/2019 Mechanical Properties of Materials.pdf

10/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-10

3.49 The pins in the truss shown in Fig. P3.49are displaced by u

and v in the x and y direction respectively, as given. All rods in the truss

have an area of cross-section A= 100 mm2 and a Modulus of Elasticity

E= 200 GPa.

uA 4.6765 mm= vA 0=

uB 3.3775 mm= vB 8.8793 mm=

uC 2.0785 mm= vC 9.7657 mm=

uD 1.0392 mm= vD 8.4118 mm=

uE 0.0000 mm= vE 0.0000 mm=

uF 3.260 0 mm= vF 8.4118 mm=

uG 2.5382 mm= vG 9.2461 mm=

uH 1.5500 mm= vH 8.8793 mm=

Determine the external force P4and P5 in the truss shown in Fig. P3.49

P4

P3

P2

P1

300 300

3 m 3 m 3 m 3 m

A B C D E

F

G

HP5

x

y

Fig. P3.49

• 8/10/2019 Mechanical Properties of Materials.pdf

11/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-11

Isotropy and Homogeneity

Linear relationship between stress and strain components:

xx C11xx C12yy C13zz C14yz C15zx C16xy+ + + + +=yy C21xx C22yy C23zz C24yz C25zx C26xy+ + + + +=

zz C31xx C32yy C33zz C34yz C35zx C36xy+ + + + +=

yz C41xx C42yy C43zz C44yz C45zx C46xy+ + + + +=

zx C51xx C52yy C53zz C54yz C55zx C56xy+ + + + +=

xy C61xx C62yy C63zz C64yz C65zx C66xy+ + + + += An isotropic materialhas a stress-strain relationships that are inde-

pendent of the orientation of the coordinate system at a point.

A material is said to be homogenousif the material properties are thesame at all points in the body. Alternatively, if the material constants

Cijare functions of the coordinates x, y, or z, then the material is called

non-homogenous.

For Isotropic Materials: G E

2 1 +( )--------------------=

• 8/10/2019 Mechanical Properties of Materials.pdf

12/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-12

Generalized Hookes Law for Isotropic

Materials

The relationship between stresses and strains in three-dimensions iscalled the Generalized Hookes Law.

xx

xx

yy

zz

+( )[ ] E=

yy

yy

zz

xx

+( )[ ] E=

zz

zz

xx

yy

+( )[ ] E=

xy

xy

G=

yz

yz

G=

zx

zx

G=

G E

2 1 +( )--------------------=

xx

yy

zz

1

E------

1 1 1

xx

yy

zz

=

• 8/10/2019 Mechanical Properties of Materials.pdf

13/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-13

Plane Stress and Plane Strain

Plane Stress

Plane Strain

GeneralizedHookes Law

GeneralizedHookes Law

xx xy 0yx yy 0

0 0 0

xx xy 0yx yy 0

0 0 zzE--- xx yy+( )=

xx xy 0

yx yy 0

0 0 0

xx xy 0

yx yy 0

0 0 zz xx yy+( )=

Plane Stress Plane Strain

• 8/10/2019 Mechanical Properties of Materials.pdf

14/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-14

3.78 A 2in x 2 in square with a circle inscribed is stressed as shown

Fig. P3.78. The plate material has a Modulus of Elasticity of

E = 10,000 ksi and a Poissons ratio= 0.25. Assuming plane stress,determine the major and minor axis of the ellipse formed due to deforma-

tion.

20 ksi

10 ksi

Fig. P3.78

Class Problem 1

The stress components at a point are as given.

Determine xx assuming (a) Plane stress (b) Plane strain

xx 100 MPa T( )=

yy 200 MPa C( )=

xy 125 MPa=

E 200 GPa=

0.25=

• 8/10/2019 Mechanical Properties of Materials.pdf

15/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-15

Failure and factor of safety

Failure implies that a component or a structure does not perform the

function it was designed for.

Ksafety

Failure producing value

Computed allowable( )value-------------------------------------------------------------------------= 3.1

• 8/10/2019 Mechanical Properties of Materials.pdf

16/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3-16

3.106 An adhesively bonded joint in wood is fabricated as shown.

For a factor of safety of 1.25, determine the minimum overlap length L

and dimension h to the nearest 1/8th inch. The shear strength of adhesive

is 400 psi and the wood strength is 6 ksi in tension.

L

8 in

h

hh

10 kips10 kips

Fig. P3.106

• 8/10/2019 Mechanical Properties of Materials.pdf

17/17

M. Vable Mechanics of Materials: Chapter 3 Oxford University Press

3 17

Common Limitations to Theories in

Chapter 4-7

The length of the member is significantly greater (approximately 10times) then the greatest dimension in the cross-section.

We are away from regions of stress concentration, where displace-

ments and stresses can be three-dimensional.

The variation of external loads or changes in the cross-sectional area is

gradual except in regions of stress concentration.

The external loads are such that the axial, torsion and bending prob-

lems can be studied individually.

http://../Book/Introduction/axial.pdfhttp://../Book/Introduction/axial.pdf

Recommended